7 Hardened Concrete
Embed Size (px)
Transcript of 7 Hardened Concrete
HARDENED CONCRETE Total 31 1
Shrinkage Shrinkage of concrete is caused by the settlement of solids and the loss of free water from the plastic concrete (plastic shrinkage),
by the chemical combination of cement with water (autogenous shrinkage) and
by the drying concrete (drying shrinkage).
CRACKING: Where movement of the concrete is restrained, shrinkage will produce tensile stress within the concrete, which may cause cracking.
Total 31 2
Plastic Shrinkage Shrinkage, which takes place before concrete has set, is
known as plastic shrinkage. Occurs as a result of the loss of free water and the settlement of solids
in the mix.
Plastic shrinkage is most common in slab construction and is characterized by the appearance of surface cracks which can extend quite deeply into the concrete.
Preventive measures: Reduce water loss by any curing methods (cover concrete
with wet polythene sheets or by spraying a membrane-curing compound).
Total 31 3
Total 31 4
Plastic Shrinkage Cracks
Total 31 5
As hydration continues in an environment where the water content is constant, such as inside a large mass of concrete, this decrease in volume of the cement paste results in shrinkage of the concrete.
This is known as autogenous shrinkage, it is self-produced by the hydration of cement. Factors influencing the rate and magnitude of autogenous
Chemical composition of cement, Initial water content, Temperature and time. Total 31 6
When a hardened concrete, cured in water, is allowed to dry it first loses water from its voids and capillary pores and only starts to shrink during further drying when water is drawn, out of its cement gel. This is known as drying shrinkage.
After an initial high rate of drying shrinkage concrete continues to shrink for a long period of time, but at a continuously decreasing rate.
For practical purposes, it may be assumed that for small sections 50 per cent of the total shrinkage occurs in the first year.
Total 31 7
Drying Shrinkage Cracks
Total 31 8
Factors Affecting Drying Shrinkage
Type, content and proportion of the constituent materials of
concrete (cement, water, aggregates, etc), Size and shape of the concrete structure, Amount and distribution of reinforcement, Relative humidity of the environment.
Drying shrinkage is directly proportional to the water-cement ratio and inversely proportional to the aggregate-cement ratio (Figure 1). Because of the interaction of the effects of aggregate-cement and water-cement ratios, it is possible to have a rich mix with a low water-cement ratio giving higher shrinkage than a leaner mix with a higher water-cement ratio.
Total 31 9
Figure 1. Influence of water/cement ratio and aggregate content on shrinkage.
Total 31 10
The durability of concrete can be defined as its resistance to deterioration resulting from external and internal causes.
Total 31 11
Factors Affecting Durability
Physical, chemical or mechanical: a) Leaching out of cement (Ca(OH)2)
b) Actions of sulphates, seawater and natural slightly acidic water. The resistance to these attacks varies with the type of cement used and increases in the order; OPC and RHC (rapid hardening cement)
Environmental such as occurrence of extreme temperatures, abrasion and electrostatic action.
Attack by natural or industrial liquids and gasses.
Total 31 12
1. Alkali-aggregate reactions
2. Volume change due to difference in thermal properties of the aggregate and cement paste.
3. Permeability of concrete.
Is the reactions between the active SILICA constituents of the aggregate, and ALKALIES in cement. As a result of these reactions expansion of cement gel causes cracks.
Reactive form of SILICA occurs in OPALINE.
Total 31 13
Recommended Protective Treatments: Low w/c ratios (less than 0.5)
Proper placing and compaction
Adequate and timely curing.
Total 31 14
Testing of Hardened Concrete
Compressive Strength Most important property of hardened concrete. Generally
considered in the design of concrete mixtures. Dimensions of the concrete specimens usually have the
following sizes: Cylindrical specimens : 7.5, 10, 15 cm diameters Cube specimens : 5, 10, 15 cm Compressive strength is affected by many factors
(environmental, curing condition). Therefore, the actual strength of concrete will not be the same as the strength of specimen.
Total 31 15
Cube & Cylinder Samples
Total 31 16
a = 5, 10, 15 cm Diameter = 7.5, 10, 15 cm
Testing for Compressive Strength
cylindrical / cube specimens.
Empty moulds are filled with fresh concrete using a standard procedure. After 24 hours the specimens are taken out of the moulds and moist cured for 28 days at the end of the curing period they are tested.
Total 31 17
P = failure load
D = diameter of cylinder
a = one side of cube
Total 31 18
Pf c 2
Cube (100, 150, 200 mm)
Cylinder 100x200 or 150x300 mm
Testing concrete for compression
Total 31 19
Materials of Construction Lab-Civil Eng. Dept.
100 mm cube
150 mm cube
200 mm cube
150x300 mm cylinder
100 mm cube 1 1.01 1.05 1.22
150 mm cube - 1.00 1.04 1.20
200 mm cube - - 1.00 1.15
100x200 mm cylinder - - - 1.06
Total 31 20
28-Day Cylinder compressive strengths of concrete classes C14-C35
Minimum Mean Strength
C14 14 18 11 17
C16 16 20 13 19
C18 18 - 14 22
C20 20 26 17 23
C25 25 31 22 28
C30 30 36 27 33
C35 35 43 32 38
21 Total 31
Microcracking & stress-strain relation
22 Total 31
Strains in a prism tested to failure in compression
23 Total 31
Stress-strain relation with constant strain rate. Testing machine is controlling the strain
24 Total 31
The tensile strength of concrete is important to resist
cracking from shrinkage and temperature changes. a) Direct Tensile Strength: Difficult to measure and is not usually done. b) Splitting Tensile Strength: The cylindrical specimens (on cube) (placed with its
axis horizontal) is subjected to a line load (uniform) along the length of the specimen (Figure 4).
Total 31 25
Total 31 26
sp = 2P/ D L
sp = 0.519 P/s2
sp = 0.642 P/s2
Figure 4 Splitting tensile test styles.
Splitting tensile strength
l : length of cylinder
d : diameter of cylinder
P: Failure load
sp : splitting tensile strength (10% of compressive strength)
Total 31 27
Problems on Hardened Concrete (compressive strength)
Sample size (mm) Failure load
calculation Compressive strength (MPa)
Cube (100x100x100 300 300 000/100x100 30.00
560 560 000/150x150 24.88
Cylinder (100x200) 730 4x730 000/3.14x100x100 93.00
Cylinder (150x300) 850 4x850 000/3.14x150x150 48.00
Total 31 28
Problems on Hardened Concrete (splitting tensile strength)
Style of Splitting
calculation Splitting tensile strength (MPa)
Normal Cube 100 150 0.642x150 000/100x100 9.63
Normal Cube 150 185 0.642x185 000/150x150 5.27
diagonal Cube 150 250 0.519x250 000/150x150 5.76
normal Cyl. 150x300 375 2x375 000/3.14x300x150 5.30
29 Total 31
1. 1. The 150 mm cubic concrete specimen is crushed under an axial
compressive load of 778 kN at 28 days age. Estimate the 28-day 150x300 mm cylinder compressive strength of the same concrete.
2. 2. A 200 mm cubic concrete specimen is crushed under a compressive load of 641 kN. Calculate the compressive load necessary to crush a 150x300 mm cylindrical specimen prepared from the same mix tested at the same age.
3. Three 150 mm cubic concrete specimens prepared from the same mix were crushed under uniaxial compressive loads of 560 kN, 570 kN and 558 kN. Calculate the average compressive strength of concrete. If the split tensile strength of concrete is 15% that of the average compressive strength, what will be minimum split tensile load necessary to crush the same cubic specimens.
Total 31 30